- ASTM 12Q Valve
- ASTM 12Q Flange
- ASTM 12Q pipe fitting
- ASTM 12Q angle bar
- ASTM 12Q pipe
Data center describes many of the common steel models, we can not determine the company's warehouse has all types of steel products inventory or raw materials.
Steel Pipe: 1 - 1300mm, also can be customed.
Pipe fitting Size: 1/8 inch - 80 inch (DN6 - DN2000)
Flange Size: DN6 - DN2000
Lenth: Any lenth based on the customer's requirement.
ASTM 12Q properties and heat treatment forged piece, Including ASTM 12Q application and specifications, Including ASTM 12Q tube plate, ASTM 12Q tube sheet, ASTM 12Q Pipe fittings, ASTM 12Q flat bar,ASTM 12Q Valve,ASTM 12Q forgings.
ASTM 12Q has the following specifications:
Chemical composition % of the ladle analysis of grade ASTM 12Q and Standards
ASTM 12Q the mechanical properties of the report, the report provides detailed performance analysis and application.
Principal Design Features
One of the most widely used precipitation hardening grades in the business. While soft and ductile in the solution annealed condition, it is capable of high properties with a single precipitation or aging treatment. Characterized by good corrosion resistance, high harness, toughness and strength.
Long, gummy chips characterize this alloys machinability. It can be machined in the annealed condition, however condition H1150M will yield best results. Post machining solution treatment of parts will be required prior to final hardening if machining in this condition.
CONDITION A--Soak at 1900 F (1038 C) for 30 minutes and cool below 60 F (16 C) for complete martensite transformation. CONDITION H 950- Treat Condition A material at 900 F(482 C) for 1 hour, air cool.. CONDITION H925, H1025, H1075, H1100, H1150- Soak solution treated material for 4 hours at specified temperature, air cool, CONDITION H1150M- Soak solution treated material at 1400 F (760 C) for 2 hours, air cool, then re-heat to 1150 F (620 C) for 4 hours and air cool.
Successfully welded by common fusion and resistance methods, this alloy should not be joined by oxyacetylene welding. AWS E/ER630 filler metal is recommended if required.
Soak for 1 hour at 2150 F (1177 C) prior to forging. Do not work below 1850 F (1010 C). Post-work solution treatment is required prior to final hardening.